| Abstract|| |
Efficient endodontic treatment demands thorough debridement of the root canal system with minimal procedural errors. The inherent weakness of nickel–titanium alloys is their unexpected breakage. Modifications in the design, manufacturing, thermomechanical and surface treatment of alloys and advancements in movement kinetics have shown to improve the fatigue properties of the alloys, reducing the incidence of separation. This review enlightens the impact of these factors on fatigue properties of the alloy.
Keywords: Fatigue properties; movement kinetics; rotary design; thermally treated alloys
|How to cite this article:|
Khasnis SA, Kar PP, Kamal A, Patil JD. Rotary science and its impact on instrument separation: A focused review. J Conserv Dent 2018;21:116-24
|How to cite this URL:|
Khasnis SA, Kar PP, Kamal A, Patil JD. Rotary science and its impact on instrument separation: A focused review. J Conserv Dent [serial online] 2018 [cited 2018 Apr 19];21:116-24. Available from: http://www.jcd.org.in/text.asp?2018/21/2/116/228265
| Introduction|| |
Separation of rotary nickel–titanium (RNT) has been an enigma to endodontists and practitioners since their introduction by Walia et al. in 1988. The reported incidence of separation of RNT is 1.3%–10% in the literature,, 44.3% of which are attributed to cyclic fatigue and 55.7% to torsional failure. Cyclic or flexural fatigue occurs when the instrument rotates freely in a curved canal, with repeated compression/tension cycles to the point of maximum flexure to cause fracture of the instrument. Torsional fatigue failure occurs in a narrow canal, when the tip of a rotary file binds while the shank of the handpiece continues to rotate exceeding the elastic limit of the file. Separated instrument compromises disinfection and obturation protocols, leading to failure of endodontic treatment. Removal of RNT is not only challenging, but none of the retrieval systems ensure 100% success rate.
Hence, “To prevent rather to treat the breakage” is the dictum among the clinicians. Improvements in instrument design, manufacturing process, and movement kinetics have been attempted to reduce the risk of separation. This review provides an insight into scientific causes of instrument separation, prevention strategies, and clinical recommendations for safer and efficient rotary endodontics.
| Materials and Methods|| |
An electronic search was carried out using the following keywords: “cyclic fatigue/torsional resistance of NiTi rotary” to collect literature, from Journal of Endodontics, International and Australian Endodontic Journal, Journal of Conservative Dentistry, Endodontic Topics, from 2000-2017 July. The abstracts and full text of relevant articles were obtained to collect comprehensive update on instrument separation.
| Discussion|| |
The review is discussed under the following headings:
- Ruddle's classification
- Nickel–titanium (NiTi) metallurgy, phase transformation, and properties
- Factors influencing separation
- Canal curvature
- Manufacturing process, heat and surface treatments
- Rotary design which includes cross section, tip, taper, pitch, radial land, rake angle, and helical angle
- Movement kinetics which includes torque, rotational speed, rotation, reciprocation, and adaptive motion.
Cyclic fatigue resistance (CFR), torsional resistance (TR), superelasticity (SE), shape memory (SM).
Clifford Ruddle's classification of evolution of rotary instruments
First generation (the mid to late 90s)
Rotary files with passive cutting radial lands and fixed taper such as 4% and 6% over the length of their cutting blades are included. For example, profiles 0.04 and 0.06.
Second generation (2001)
Files with active cutting edges, alternating cutting points, multiple tapers on a single file and electropolished files are included; for example: RaCe, EndoSequence and ProTaper.
Third generation (2007)
Thermally treated alloys mark this generation. These alloys exhibited superior flexibility and remarkable fatigue resistance; for example: Twisted File, HyFlex ® CM, and ProfileVortex.
Fourth generation (2008)
Introduction of reciprocation concept: Endo EZE, M4, and reciprocating handpieces use equal clockwise/counterclockwise angles of 300. Yared et al. advocated unequal angles of reciprocation; For example: Wave One and Reciproc. Self-adjusting files by ReDent Nova, with new design and mode of operation, serve as a conservative approach for root canal preparation.
Files with offset designs to reduce the screwing in and breakage mark the fifth generation; for example; ProTaper Next and Revo-S.
Equiatomic NiTi has 56% Ni and 44% Ti. At this ratio, NiTi alloys exhibit SE and SM. While SE endows the file with superior flexibility to negotiate canal curvatures, SM allows the file regain its original shape. The surface of RNT has metallic nickel, oxygen, carbon, and oxides of NiTi. Decrease in the nickel content improves the fatigue resistance of NiTi alloys. HyFlex ® has 52 wt% Ni (conventional RNT has 54%wt–57%wt), which lowers the Af to 47°C.
Phase transformation and properties
Clinically, NiTi exists as one of the three phases: austenite, martensite, and an intermediate R-Phase. Their interconversion is a reversible phenomenon and is a function of temperature and stress [Figure 1]. Transformation temperature is influenced by the composition, impurities, and heat treatment of the alloy, which in turn influences its mechanical properties  [Figure 2].
|Figure 1: (a) Phase transformation of nickel–titanium alloy; As: Austenitic start, Af: Austenitic finish, Ms: Martensitic start, Mf: Martensitic finish. (b) Properties of conventional rotary nickel–titanium (i) Conventional rotary file exhibiting (ii) superelasticity when stressed in the canal, (iii) shape memory when the stress is released. (c) Properties of thermally treated rotary nickel–titanium alloy (i) Controlled memory file, exhibiting (ii) superelasticity (iii) but no shape memory when stress is released, also (iv) deformation under stress and (v) regains shape on heating|
Click here to view
|Figure 2: Impact of phase transformation on the properties of nickel–titanium alloys|
Click here to view
Factors influencing the separation of rotary files
Various factors have an impact on the fatigue properties of rotary NiTi instruments [Table 2].
|Table 2: Impact of various factors on cyclic fatigue and torsional resistance: A report of studies from 2010 to 2017|
Click here to view
Fracture of instruments occurs commonly in the apical one-third where torsional and flexural stresses are highest. Hence, torsional and bending tests are performed at D3. A flexible file has more CFR but less TR and enables a smoother preparation in curved canals without being deformed. Whereas, a rigid file would be good in torsion than in flexion and performs better in narrow, constricted canals. Thus, cyclic and torsional properties are in inverse relationship with each other.
As the radius of curvature of canal increases, the frequency for instrument separation increases. A canal with 50° curvature gives rise to stress of about 700–800 MPa on the outermost part of the instrument, whereas ultimate tensile strength of NiTi is 1400 MPa.
Grinding versus twisting: In grinding, NiTi is cut across grain of the crystalline structure which causes grooves and microcracks, leading to stress concentration. To release these stresses or crystalline defects, annealing heat treatment is given. It increases the flexibility and modifies the phase transformation behavior.
Thermal treatment of alloys
R-phase alloys have more flexibility, TR  and CFR  than conventional alloys with the same geometry, in both dry and aqueous environments, and also when used in reciprocating motion. However, they have low TR than M-wire alloys.
They are produced by a series of heat treatment and annealing cycles which endow them superior strength due to stable nanocrystalline martensitic structure.
Controlled Memory Alloys
Unlike conventional rotary files, controlled memory files do not exhibit SM, and hence do not straighten the canal or cause ledging [Figure 1]b, [Figure 1]c and [Figure 2]. Instruments with low transformation temperature exhibit (Hero, K3) higher maximum torque and resist fracture better than instruments with high transformation temperature (Endowave, Profile, and ProTaper).
Alloys With Gold Thermal Treatment
Files are subjected to a temperature of 370°C–510°C for 10–60 min depending on the size and taper of files. Files exhibit two-stage transformation behavior and high Af temperature of 50°C; for example ProTaper Gold.
In WaveOne Gold, a constant strain of 3–15 kg is applied at a temperature of 410°C–440°C. After machining, the working portion is again heat treated at 120°C–260°C.
Maxwire Alloys (Martensite-Austenite Electropolish Flex) Alloys
This new technology allows the file XPendoShaper to attain martensitic phase when cooled (20°C) and austenitic phase at body temperature (37°C). At austenitic phase, it has a snake-like shape adapting to the canal irregularities, reducing stress on the file.
The proprietary heat treatment claims to increase the flexibility and fracture resistance by 40%; for example: 2 shape files, it has two rotary files TS1 and TS2. The instruments regain their original shape after each use.
Thermally treated alloys have low modulus of elasticity (20–40 GPa) than conventional (40–90 GPa) alloys and resist fracture better under stress.
Surface treatment of nickel–titanium alloys
Rotary files are subjected to various surface treatments to improve their properties [Table 1]. Implantation of Argon ion increases the fatigue resistance. Nitrogen ion implantation has negative effect on fatigue resistance. Thermal nitridation at 250°C has shown more fatigue resistance because at 300°C the superelastic behavior is lost. Deep dry cryogenic treatment of 24 h, at −185°C, provides adequate time for transformation of retained austenite to martensite, improving the fatigue life., Electropolished instruments have more number of cycles to fracture than that of nonpolished instruments. However, it does not prevent the development of microcracks on the instrument surface.,
|Table 1: Impact of surface treatment on properties of nickel-titanium alloys|
Click here to view
Electric discharge machining technology
Electric discharge machining (EDM) technology is a noncontact thermal erosion process in which electric sparks are used to melt and vaporize the top layer of NiTi alloy, reducing the surface defects. This increases the fracture resistance of files. After cutting, cleaning is done ultrasonically in an acid bath. Then, they are heat treated at 300°C–600°C for 10 min, 5 h before and after the cleaning; for example: HyFlex ® EDM
Blue phase treatment
In this, the surface of a NiTi alloy is treated with titanium oxide by proprietary manufacturing process, which increases the surface hardness, wear resistance, cutting efficiency and flexibility of the file; for example: Vortex Blue and Reciproc Blue.
Design features related to instrument separation
Rotary files are manufactured with different cross-sectional designs; for example: Convex triangle-ProTaper, Wave One, Triple U-Profile, Equilateral triangle-Race, S-type-M-two, Reciproc, and Rectangular–ProTaper Next
- Inner core and CSA: More the core and CSA, more is the TR but less is the CFR.,, This is the reason for improved fracture resistance of ProTapers than profiles in narrow canals 
- Cross-sectional design: Instrument separation occurs in the decreasing order with the following cross sections
- Square > rectangular > triangular and slender rectangular triangle ,
- S-shaped, H-file fracture more compared to triangular cross section 
- Alloy type: With the same cross section, M-wire alloy resists fracture better than conventional alloy 
- Different cross sections along the length of an instrument improve the fracture resistance; for example: One shape and WaveOne 
- Asymmetric cross sections of ProTaper Next and Revo-S also reduce screwing in and breakage 
- Protaper universal files (F2, F3, F4, F5) are made more flexible by incorporating an additional groove in the middle of side of convex triangular cross section.,
In general, NiTi rotary instruments are designed with noncutting tips to prevent ledging, torsional failure, and fracture.
Booster tip is a lead tip, that is incorporated in XPendoShaper. The lead section enters canal ensuring fit into the pre-established glide path. There are no cutting flutes on this section (¼ mm) where as the next ¼ mm has 6 cutting flutes, which shapes canal to #25/.02 to #60/.02 instrument. The repeated use of the shaper prepares the canal to a taper size consistent with the intracanal dentinal anatomy and hardness.
Taper is increase in the diameter of file per mm increase in length. Fixed taper files cause excessive screwing in and taper lock than graduating or variable taper files.,, An instrument with larger taper and tip diameter is more likely to fracture in a canal with more acute and coronally located curvature.
It refers to the number of flutes per unit length of the file. More the flutes on the file, lesser the pitch and more is the fracture resistance of the file. Hence, it is recommended to use a file with smaller pitch (more flutes) for both curved and straight canals.
Radial land is a surface that projects axially from the central axis between the flutes, it as far as the cutting edges. Increased width of land increases the peripheral strength and canal-centering ability, but induces stresses due to increased contact with the canal wall causing fracture. To balance these properties, K3 is designed with two recessed and one full land: ProTaper and Race lack radial lands.
It is the angle formed by the cutting edge and cross-section taken perpendicular to the long axis of the instrument. Slight positive rake angle is recommended to for both good cutting action and reduced screwing in; for example: K3.
Helical angle is the angle that the cutting edge makes with the long axis of the file. Varying the helical angle through the working part has been shown to reduce the screwing in tendency; for example; in K3, helical angle is increased from tip to the handle. In Race, alternate helical design reduces the torque.
It is the force that is exerted on an object in rotation. It is measured in gram centimeters.
In endodontics, torque is related to the apically directed force and preoperative canal volume.
Conventional or slow-speed, high-torque motors (>3 Ncm) cause fracture of instruments in curved canals. Slow-speed, low-torque motors provide the right torque for the specific file.
The values are smaller (low torque) for smaller and less tapered instruments and higher (high torque) for bigger and more tapered instrument.
Optimum torque reverse
It is based on the principle of torque-provoked reversal, which is activated when preset torque is exceeded during 1800 forward rotation, and then the file rotates backward 900 to release itself. It provides high cutting effectiveness at very low torque values and moderate speed. Files have shown better fatigue resistance in Optimum Torque Reverse (OTR) motors.
Safety quotient = RFT/MWT.
Where RFT – “Rotation to failure torque” is measured by turning a file that has been grasped and immobilized at D3 at a constant revolutions per minute (rpm).
MWT – “Mean working torque”– the torque required for any given NiTi to cut the dentin.
Ideally, safety quotient should be greater than one to reduce the risk of file fracture.
Higher is the torque, greater is the breakage. Torque is higher in the following:
- Narrower canals, large diameter file,,, acute canal curvature, and rotary instrumentation without glidepath.
Rotational speed (revolutions per minute)
The recommended rpm for most of the rotary files is between 250–500 rpm.
Higher speed causes increased fracture of files due to the following:
- Increased stress  and strain rate and decreased time for stress relaxation
- Increased chance for taper lock 
- More heat is generated during conversion of austenite to martensite, leading to precocious fatigue of the metal.
The inverse relationship between speed and torque
As speed increases, torque decreases, which compensates for negative effect of increased speed on cyclic fatigue. Hence, endodontic handpieces deliver low speeds for higher working torque for the individual file to reduce separation.
Rotation, reciprocation, and adaptive motion
It is continuous clockwise rotation of file. Rotary files undergo plastic deformation when their endurance limit is exceeded. Endurance limit is the level of stress or strain at which a file can be subjected to a virtual infinite cycles without failure.
It is defined as repeated CW/CCW movements of the file. Reciprocation can be as follows:
- Complete: Reciprocating angles are same in both CW and CCW directions
- Partial: It has angles of 3700 in cutting verse CW and 500 noncutting verse CCW
- Hybrid reciprocation: Here, the angles change depending on the intracanal torque.
In reciprocation, the CW rotation changes to CCW before the file is subjected to endurance limit, hence reducing the risk of separation. The reasons include, in reciprocation, fatigue of file occurs at multiple sites, whereas in rotary, a single site undergoes repeated fatigue. During one reciprocation, i.e., CW/CCW motion, crack formed in the file opens and closes once. A higher number of reciprocating cycles are required to complete one full rotation, which extends the CFR.
Heat treatment  and reciprocating motion have been shown to enhance the CFR of some rotary files, such as ProTaper F2 and K3XF.
The feature of this motor is that it changes kinematics from an interrupted complete rotating movement (6000 CW and 00 CCW) to a partial reciprocation (3700 CW/ 500 CCW) according to the intracanal pressure. Adaptive motion does not improve the CFR.
Other factors affecting fracture resistance
Fracture resistance is not affected by autoclaving of new files in vitro, unlike during clinical use. CM and R-phase alloys exhibited increased CFR on autoclaving.
A rotary file is often subjected to a combination of torsional and cyclic stresses in the canal.In vitro studies have shown that torsional preloads increase the fatigue, but improve torsional strength, where as cyclic preloads add to tosional failure.
Clinical recommendations for a safer rotary
- A generous access with flexible files for severe curvatures and stiffer ones for straight canals
- Stick to the rpm and torque as recommended, no high rpm for curvatures
- Secure a patent glidepath. It takes off that extra torque on the files
- Lubrication and light touch, follow the sequence of files
- Monitor the files before reuse, there is no SAFE NUMBER
- Pecking motion for radial landed and brushing motion for nonlanded files 
- Lateral brushing motion for oval canals 
- Small taper and tip diameter file for more coronal and/or acute curves 
- Be selective for single-visit cases
- Practice hybrid instrumentation, i.e., more than one rotary system for individual case.
| Conclusion|| |
Selection of proper file by the clinician, for the individual case, would balance the conflict between fatigue properties of the alloy, enabling a more efficient preparation of the canal with reduced risk of separation.
I would like to acknowledge Dr. Shrinivas S Vanaki, Principal, PMNM Dental College, Bagalkot, for his constant support and encouragement for the research work.
Also, I would like to thank Mr. Kotambari and Mr. Vijay, Chief Librarians, for providing us with unmatching library facilities for this exhaustive piece of research work.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Walia HM, Brantley WA, Gerstein H. An initial investigation of the bending and torsional properties of Nitinol root canal files. J Endod 1988;14:346-51.
Iqbal MK, Kohli MR, Kim JS. A retrospective clinical study of incidence of root canal instrument separation in an endodontics graduate program: A PennEndo database study. J Endod 2006;32:1048-52.
Spili P, Parashos P, Messer HH. The impact of instrument fracture on outcome of endodontic treatment. J Endod 2005;31:845-50.
Sattapan B, Nervo GJ, Palamara JE, Messer HH. Defects in rotary nickel-titanium files after clinical use. J Endod 2000;26:161-5.
Siqueira JF Jr. Aetiology of root canal treatment failure: Why well-treated teeth can fail. Int Endod J 2001;34:1-0.
Gencoglu N, Helvacioglu D. Comparison of the different techniques to remove fractured endodontic instruments from root canal systems. Eur J Dent 2009;3:90-5.
Ruddle CJ, Machtou P, West JD. The shaping movement: Fifth-generation technology. Dent Today 2013;32:94, 96-9.
Mohammadi Z, Soltani MK, Shalavi S, Asgary S. A review of the various surface treatments of NiTi instruments. Iran Endod J 2014;9:235-40.
Testarelli L, Plotino G, Al-Sudani D, Vincenzi V, Giansiracusa A, Grande NM, et al.
Bending properties of a new nickel-titanium alloy with a lower percent by weight of nickel. J Endod 2011;37:1293-5.
Shen Y, Zhou HM, Zheng YF, Peng B, Haapasalo M. Current challenges and concepts of the thermomechanical treatment of nickel-titanium instruments. J Endod 2013;39:163-72.
Braga LC, Magalhães RR, Nakagawa RK, Puente CG, Buono VT, Bahia MG, et al.
Physical and mechanical properties of twisted or ground nickel-titanium instruments. Int Endod J 2013;46:458-65.
Baek SH, Lee CJ, Versluis A, Kim BM, Lee W, Kim HC, et al.
Comparison of torsional stiffness of nickel-titanium rotary files with different geometric characteristics. J Endod 2011;37:1283-6.
Martin B, Zelada G, Varela P, Babillio JG, Magan F, Ahn S, et al
. Factors influencing the fracture of niTi rotary instruments. Int Endod J 2003;36:1394-8.
Zhang EW, Cheung GS, Zheng YF. Influence of cross-sectional design and dimension on mechanical behavior of nickel-titanium instruments under torsion and bending: A numerical analysis. J Endod 2010;36:1394-8.
Kim HC, Yum J, Hur B, Cheung GS. Cyclic fatigue and fracture characteristics of ground and twisted nickel-titanium rotary files. J Endod 2010;36:147-52.
Ebihara A, Yahata Y, Miyara K, Nakano K, Hayashi Y, Suda H, et al.
Heat treatment of nickel-titanium rotary endodontic instruments: Effects on bending properties and shaping abilities. Int Endod J 2011;44:843-9.
Larsen CM, Watanabe I, Glickman GN, He J. Cyclic fatigue analysis of a new generation of nickel titanium rotary instruments. J Endod 2009;35:401-3.
Shen Y, Zhou H, Campbell L, Wang Z, Wang R, Du T, et al.
Fatigue and nanomechanical properties of K3XF nickel-titanium instruments. Int Endod J 2014;47:1160-7.
Pérez-Higueras JJ, Arias A, de la Macorra JC. Cyclic fatigue resistance of K3, K3XF, and twisted file nickel-titanium files under continuous rotation or reciprocating motion. J Endod 2013;39:1585-8.
Elnaghy AM, Elsaka SE. Assessment of the mechanical properties of proTaper next nickel-titanium rotary files. J Endod 2014;40:1830-4.
Zhou H, Peng B, Zheng Y. An overview of mechanical properties of nickel-titanium endodontic instruments. Endod Topics 2013;29:42-54.
Aoun CM, Nehme WB, Naamanand AS, Khalil IT. Review and classification of heat treatment procedures and their impact on mechanical behaviour of endodontic files. Int J Curr Res 2017;9:51300-6.
Silva EJ, Vieira VT, Belladonna FG, Zuolo AS, Antunes HD, Cavalcante DM, et al.
Cyclic and torsional fatigue resistance of XP-endo shaper and TRUShape instruments. J Endod 2017. pii: S0099-2399(17) 31034-8.
Vinothkumar TS, Kandaswamy D, Prabhakaran G, Rajadurai A. Microstructure of cryogenically treated martensitic shape memory nickel-titanium alloy. J Conserv Dent 2015;18:292-6.
] [Full text]
Vinothkumar TS, Kandaswamy D, Prabhakaran G, Rajadurai A. Mechanical behavior of deep cryogenically treated martensitic shape memory nickel-titanium rotary endodontic instruments. Eur J Dent 2016;10:183-7. [Full text]
Anderson ME, Price JW, Parashos P. Fracture resistance of electropolished rotary nickel-titanium endodontic instruments. J Endod 2007;33:1212-6.
Pedulla E, La Savio F, Boninelli S, Plotino G, Grande NM, La Rosa G, et al
. Torsional and cyclic fatigue resistance of NiTi instruments manufactured by electric discharge machining. J Endod 2016;42:156-9.
Xu X, Eng M, Zheng Y, Eng D. Comparative study of torsional and bending properties for six models of nickel-titanium root canal instruments with different cross-sections. J Endod 2006;32:372-5.
Schäfer E, Dzepina A, Danesh G. Bending properties of rotary nickel-titanium instruments. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2003;96:757-63.
Subramaniam V, Indira R, Srinivasan MR, Shankar P. Stress distribution in rotary NiTi instruments – A finite element analysis. J Cons Endod 2007;10:112-8.
Ha JH, Cheung GS, Versluis A, Lee CJ, Kwak SW, Kim HC, et al.
'Screw-in' tendency of rotary nickel-titanium files due to design geometry. Int Endod J 2015;48:666-72.
Kim HC, Kim HJ, Lee CJ, Kim BM, Park JK, Versluis A, et al.
Mechanical response of nickel-titanium instruments with different cross-sectional designs during shaping of simulated curved canals. Int Endod J 2009;42:593-602.
Park SY, Cheung GS, Yum J, Hur B, Park JK, Kim HC, et al.
Dynamic torsional resistance of nickel-titanium rotary instruments. J Endod 2010;36:1200-4.
Dagna A, Poggio C, Beltrami R, Colombo M, Chiesa M, Bianchi S, et al.
Cyclic fatigue resistance of OneShape, Reciproc, and WaveOne: An in vitro
comparative study. J Conserv Dent 2014;17:250-4.
] [Full text]
Haapasalo M, Shen Y. Evolution of Nickel titanium instruments: From past to future. Endod Topics 2013;29:3-17.
Viana AC, Chaves Craveiro de Melo M, Guiomar de Azevedo Bahia M, Lopes Buono VT. Relationship between flexibility and physical, chemical, and geometric characteristics of rotary nickel-titanium instruments. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2010;110:527-33.
Bergmans L, Van Cleynenbreugel J, Beullens M, Wevers M, Van Meerbeek B, Lambrechts P, et al.
Progressive versus constant tapered shaft design using NiTi rotary instruments. Int Endod J 2003;36:288-95.
Peters OA, Paque F. Current developments in rotary root canal instrument technology and clinical use: A review. Quintessence Int 2010;41:479-88.
Versluis A, Kim HC, Lee W, Kim BM, Lee CJ. Flexural stiffness and stresses in nickel-titanium rotary files for various pitch and cross-sectional geometries. J Endod 2012;38:1399-403.
Koch K, Brave D. Real world endo: Design features of rotary files and how they affect clinical performance. Oral Health 2002;39-49.
Gambarini G. Advantages and disadvantages of new torque controlled endodontic motors and low torque NiTi instrumentation. Aust Endod J 2001;27:99-104.
Technical report ; OTR- A new standard in mechanical root canal preparation; Available from: http://www.mbconsult2000.net
. [Last accessed on 2017 Dec 29].
Blum JY, Machtou P, Ruddle C, Micallef JP. Analysis of mechanical preparations in extracted teeth using ProTaper rotary instruments: Value of the safety quotient. J Endod 2003;29:567-75.
Bahia MG, Melo MC, Buono VT. Influence of cyclic torsional loading on the fatigue resistance of K3 instruments. Int Endod J 2008;41:883-91.
Melo MC, Pereira ES, Viana AC, Fonseca AM, Buono VT, Bahia MG, et al.
Dimensional characterization and mechanical behaviour of K3 rotary instruments. Int Endod J 2008;41:329-38.
Peters OA, Barbakow F. Dynamic torque and apical forces of proFile. 04 rotary instruments during preparation of curved canals. Int Endod J 2002;35:379-89.
Necchi S, Taschieri S, Petrini L, Migliavacca F. Mechanical behaviour of nickel-titanium rotary endodontic instruments in simulated clinical conditions: A computational study. Int Endod J 2008;41:939-49.
Peters OA, Peters CI, Schönenberger K, Barbakow F. ProTaper rotary root canal preparation: Assessment of torque and force in relation to canal anatomy. Int Endod J 2003;36:93-9.
Bardsley S, Peters CI, Peters OA. The effect of three rotational speed settings on torque and apical force with vortex rotary instruments in vitro
. J Endod 2011;37:860-4.
Lopes HP, Ferreira AA, Elias CN, Moreira EJ, de Oliveira JC, Siqueira JF Jr., et al.
Influence of rotational speed on the cyclic fatigue of rotary nickel-titanium endodontic instruments. J Endod 2009;35:1013-6.
Grande NM, Ahmed HM, Cohen S, Bukiet F, Plotino G. Current assessment of reciprocation in endodontic preparation: A comprehensive review-part I: Historic perspectives and current applications. J Endod 2015;41:1778-83.
De-Deus G, Moreira EJ, Lopes HP, Elias CN. Extended cyclic fatigue life of F2 ProTaper instruments used in reciprocating movement. Int Endod J 2010;43:1063-8.
Kiefner P, Ban M, De-Deus G. Is the reciprocating movement per se
able to improve the cyclic fatigue resistance of instruments? Int Endod J 2014;47:430-6.
Çapar ID, Arslan H. A review of instrumentation kinematics of engine-driven nickel-titanium instruments. Int Endod J 2016;49:119-35.
Ertas H, Capar ID, Arslan H. Cyclic fatigue resistance of Protaper Universal, TF -Adaptive, Reciproc and WaveOne systems. Turk Endod J 2016;1:30-4.
Arias A, Perez-Higueras JJ, De la Macorra CJ. Influence and clinical usage of GT and GTseries X files on cyclic fatigue resistance. Int Endod J 2014;47:257-63.
Zhao D, Shen Y, Peng B, Haapasalo M. Effect of autoclave sterilization on the cyclic fatigue resistance of thermally treated nickel-titanium instruments. Int Endod J 2016;49:990-5.
Pedullà E, Lo Savio F, Boninelli S, Plotino G, Grande NM, Rapisarda E, et al.
Influence of cyclic torsional preloading on cyclic fatigue resistance of nickel-titanium instruments. Int Endod J 2015;48:1043-50.
Oh SH, Ha JH, Kwak SW, Ahn SW, Lee W, Kim HC, et al.
The effects of torsional preloading on the torsional resistance of nickel-titanium instruments. J Endod 2017;43:157-62.
Kim JY, Cheung GS, Park SH, Ko DC, Kim JW, Kim HC, et al.
Effect from cyclic fatigue of nickel-titanium rotary files on torsional resistance. J Endod 2012;38:527-30.
Plotino G, Grande NM, Sorci E, Malagnino VA, Songma F. Influence of brushing working motion on the fatigue life on nickel-titanium rotary instruments. Int Endod J 2007;40:45-51.
Rodrigues RC, Lopes HP, Elias CN, Amaral G, Vieira VT, De Martin AS, et al.
Influence of different manufacturing methods on the cyclic fatigue of rotary nickel-titanium endodontic instruments. J Endod 2011;37:1553-7.
Gambarini G, Plotino G, Grande NM, Al-Sudani D, De Luca M, Testarelli L, et al.
Mechanical properties of nickel-titanium rotary instruments produced with a new manufacturing technique. Int Endod J 2011;44:337-41.
Elnaghy AM. Cyclic fatigue resistance of proTaper next nickel-titanium rotary files. Int Endod J 2014;47:1034-9.
Alcalde MP, Tanomaru-Filho M, Bramante CM, Duarte MAH, Guerreiro-Tanomaru JM, Camilo-Pinto J, et al.
Cyclic and torsional fatigue resistance of reciprocating single files manufactured by different nickel-titanium alloys. J Endod 2017;43:1186-91.
Gao Y, Shotton V, Wilkinson K, Phillips G, Johnson WB. Effects of raw material and rotational speed on the cyclic fatigue of ProFile vortex rotary instruments. J Endod 2010;36:1205-9.
Shen Y, Qian W, Abtin H, Gao Y, Haapasalo M. Fatigue testing of controlled memory wire nickel-titanium rotary instruments. J Endod 2011;37:997-1001.
Ninan E, Berzins DW. Torsion and bending properties of shape memory and superelastic nickel-titanium rotary instruments. J Endod 2013;39:101-4.
Campbell L, Shen Y, Zhou HM, Haapasalo M. Effect of fatigue on torsional failure of nickel-titanium controlled memory instruments. J Endod 2014;40:562-5.
Braga LC, Faria Silva AC, Buono VT, de Azevedo Bahia MG. Impact of heat treatments on the fatigue resistance of different rotary nickel-titanium instruments. J Endod 2014;40:1494-7.
Pereira ÉS, Viana AC, Buono VT, Peters OA, Bahia MG. Behavior of nickel-titanium instruments manufactured with different thermal treatments. J Endod 2015;41:67-71.
Bonessio N, Pereira ES, Lomiento G, Arias A, Bahia MG, Buono VT, et al
. Validated finite element analyses of Wave One endodontic instruments: A comparison between M-wire and NiTi alloys. Int Endod J 2015;48:441-50.
Capar ID, Ertas H, Arslan H. Comparison of cyclic fatigue resistance of novel nickel-titanium rotary instruments. Aust Endod J 2015;41:24-8.
Topçuoǧlu HS, Topçuoǧlu G, Akti A, Düzgün S.In vitro
comparison of cyclic fatigue resistance of ProTaper next, HyFlex CM, OneShape, and ProTaper universal instruments in a canal with a double curvature. J Endod 2016;42:969-71.
Elnaghy AM, Elsaka SE. Laboratory comparison of the mechanical properties of TRUShape with several nickel-titanium rotary instruments. Int Endod J 2017;50:805-12.
Adıgüzel M, Capar ID. Comparison of cyclic fatigue resistance of WaveOne and WaveOne gold small, primary, and large instruments. J Endod 2017;43:623-7.
Acosta EC, Resende PD, Peixoto IF, Pereira ÉS, Buono VT, Bahia MG, et al.
Influence of cyclic flexural deformation on the torsional resistance of controlled memory and conventional nickel-titanium instruments. J Endod 2017;43:613-8.
Lopes HP, Elias CN, Vieira VTL, Moreira EJL, Marques RVL, Oliveira JCM et al.
Effects of electropolishing surface treatment on the cyclic fatigue resistance of BioRace nickel titanium rotary instruments. J Endod 2010;36:1653-7
Plotino G, Grande NM, Cotti E, Testarelli L, Gambarini G. Blue treatment enhances cyclic fatigue resistance of vortex nickel-titanium rotary files. J Endod 2014;40:1451-3.
Hieawy A, Haapasalo M, Zhou H, Wang ZJ, Shen Y. Phase transformation behavior and resistance to bending and cyclic fatigue of ProTaper gold and ProTaper universal instruments. J Endod 2015;41:1134-8.
Lopes HP, Elias CN, Vieira MV, Vieira VT, de Souza LC, Dos Santos AL, et al.
Influence of surface roughness on the fatigue life of nickel-titanium rotary endodontic instruments. J Endod 2016;42:965-8.
Gündoǧar M, Özyürek T. Cyclic fatigue resistance of OneShape, HyFlex EDM, WaveOne gold, and Reciproc blue nickel-titanium instruments. J Endod 2017;43:1192-6.
da Cunha Peixoto IF, Pereira ES, da Silva JG, Viana AC, Buono VT, Bahia MG, et al.
Flexural fatigue and torsional resistance of ProFile GT and ProFile GT series X instruments. J Endod 2010;36:741-4.
Yum J, Cheung GS, Park JK, Hur B, Kim HC. Torsional strength and toughness of nickel-titanium rotary files. J Endod 2011;37:382-6.
Wycoff RC, Berzins DW. An in vitro
comparison of torsional stress properties of three different rotary nickel-titanium files with a similar cross-sectional design. J Endod 2012;38:1118-20.
Patino PV, Parraga AI, Giuseppe BR, Otero CX, Biedma BM. Alternating versus continuous rotation: A comparative study of the effect on instrument life. J Endod 2010;36:157-9.
Wan BS, Rasimick BS, Musikant BL, Deutsch AS. A comparison of cyclic fatigue resistance in reciprocating and rotary nickel titanium instruments. Aust Endod J 2011;37:122-7.
Gambarini G, Gergi R, Naceman A, Osta N, Al Sudani D. Cyclic fatigue analysis of twisted file rotary instruments used in reciprocating motion. Int Endod J 2012;45:802-6.
Kim HC, Kwak SW, Cheung GS, Ko DH, Cheung SM, Lee W. Cyclic fatigue and torsional resistance of two NiTi instruments used in reciprocation motion: Reciproc Vs Wave One. J Endod 2012;38:541-4.
Plotino G, Grande NM, Testarelli L, Gambarini G. Cyclic fatigue resistance of Reciproc and Wave One reciprocating instruments. Int Endod J 2012;45:614-8.
Gambarini G, Rubini AG, Al Sudani D, Gergi R, Culla A, D Angelis F et al
. Influence of different angles of reciprocation on the cyclic fatigue NiTi endodontic instruments. J Endod 2012; 38:1408-11.
Gambarini G, Gergi R, Grande NM, Osta N, Plotino G, Testarelli L. Cyclic fatigue resistance of newly manufactured rotary Nickel-Titanium instruments used in different rotational directions. Aust Endod J 2013;39:151-4.
Pedulla E, Grande NM, Plotino G, Gambarini G, Rapisarda E. Influence of continuous or reciprocating motion on cyclic fatigue resistance of 4 different Nickel-Titanium rotary instruments. J Endod 2013;39:258-61.
Lee WC, Hwang YJ, You SY, Kim HC. Effect of reciprocation usage of NiTi rotary files on the cyclic fatigue resistance. Aust Endod J 2013;39:146-50.
De-Deus G, Vieira VT, Da Silva EJ, Elias HL, Moreira EJ. Bending resistance and dynamic and static cyclic fatigue resistance of Reciproc and Wave One large instruments. J Endod 2014;40:575-9.
Vadhana S, Sarvanakartikeyan B, Nandini S, Velmurugan N. Cyclic fatigue resistance of Race and M-two rotary files in continuous rotation and reciprocating motions. J Endod 2014;40:995-9.
Shin CS, Huang YH, Chi CW, Lin CP. Fatigue life enhancement of NiTi rotary endodontic instruments by progressive reciprocating operation. Int Endod J 2014;47:882-8.
Higuera O, Plotino G, Tocci L, Carrillo G, Gambarini G, Jaramillo DE. Cyclic fatigue resistance of 3 different nickel-titanium reciprocating instruments in artificial canals. J Endod 2015;41:913-5.
Karatas E, Arslan H, Buker M, Seckin F, Capar ID. Effect of movement kinematics on the cyclic fatigue resistance of nickel-titanium instruments. Int Endod J 2016;49:361-4.
La Silva EJ, Villanino LS, Vieira VT, Accorsi-Mendonca T, Antunes HD, De-Deus G, et al
. Bending resistance and cyclic fatigue life of Reciproc, Unicone, and WaveOne reciprocating instruments. J Endod 2016;42:1789-93.
Arslan H, Alsancak M, Doganay E, Karatas E, Davut I, Ertas H. Cyclic fatigue analysis of Reciproc R-25 instruments with different kinematics. J Endod 2016;42:22-4.
Ozyurek T. Cyclic fatigue resistance of Reciproc, WaveOne, and WaveOne gold nickel-titanium instruments. J Endod 2016;42:1536-9.
Varghese NO, Pillai R, Sujathen UN, Sainudeen S, Antony A, Paul S. Resistance to torsional and cyclic fatigue resistance of ProTaper Next, Wave One and M-two files in continuous and reciprocating motion: An in vitro
study. J Conserv Dent 2016;19:225-30.
] [Full text]
Ferreira F, Adeodato C, Barbosa I, Aboud L, Scelza P, Scelza MZ. Movement kinematics and cyclic fatigue of NiTi titanium rotary instruments: A systematic review. Int Endod J 2017;50:143-52.
Dr. Sandhya Anand Khasnis
Department of Conservative Dentistry and Endodontics, PMNM Dental College, Bagalkot - 587 101, Karnataka
Source of Support: None, Conflict of Interest: None
[Figure 1], [Figure 2]
[Table 1], [Table 2]